Indentation hardness
Hardness measurements quantify the resistance of a material to plastic deformation. Indentation hardness tests compose the majority of processes used to determine material hardness, and can be divided into two classes: "microindentation" and "macroindentation" tests. Microindentation tests typically have forces less than . Hardness, however, cannot be considered to be a fundamental material property. Classical hardness testing usually creates a number which can be used to provide a relative idea of material properties. As such, hardness can only offer a comparative idea of the material's resistance to plastic deformation since different hardness techniques have different scales.
Vickers hardness test
It was decided that the indenter shape should be capable of producing geometrically similar impressions, irrespective of size; the impression should have well-defined points of measurement; and the indenter should have high resistance to self-deformation. A diamond in the form of a square-based pyramid satisfied these conditions. It had been established that the ideal size of a Brinell impression was of the ball diameter. As two tangents to the circle at the ends of a chord 3"d"/8 long intersect at 136°, it was decided to use this as the included angle between plane faces of the indenter tip. This gives an angle from each face normal to the horizontal plane normal of 22° on each side. The angle was varied experimentally and it was found that the hardness value obtained on a homogeneous piece of material remained constant, irrespective of load. Accordingly, loads of various magnitudes are applied to a flat surface, depending on the hardness of the material to be measured. The HV number is then determined by the ratio "F/A", where "F" is the force applied to the diamond in kilograms-force and "A" is the surface area of the resulting indentation in square millimeters. "A" can be determined by the formula.